## “

**ANALYSIS OF**

**BEHAVIOUR OF RICE HUSK ASH CEMENT CONCRETE ON **

**ADDITION OF POLYPROPYLENE FIBER”**

**Brijesh Kumar Sahu**

**1**

_{, Mr. Bhavesh Kumar Jha}

_{, Mr. Bhavesh Kumar Jha}

**2**

_{, Mr. Pukhraj Sahu}

_{, Mr. Pukhraj Sahu}

**3**

*1*

_{Student, M. Tech (Structural Engg.) GEC Jagdalpur }

_{Student, M. Tech (Structural Engg.) GEC Jagdalpur }

*2*

_{Assistant Professor, Dept. of Civil Engineering, GEC Jagdalpur, Chhattisgarh, India }

_{Assistant Professor, Dept. of Civil Engineering, GEC Jagdalpur, Chhattisgarh, India }

*3*

_{Assistant Professor, Dept. of Civil Engineering, GEC Jagdalpur, Chhattisgarh, India }

_{Assistant Professor, Dept. of Civil Engineering, GEC Jagdalpur, Chhattisgarh, India }

**---***---Abstract:-**

*The present day world is witnessing construction in*

*very challenging and difficult circumstances, where a great *
*emphasis is on sustainability. Rice husk ash and polypropylene *
*fiber, by-products of rice mill and textile industry *
*simultaneously, can enhance behaviour of concrete *
*significantly .In this experimental work the objective was to *
*study the effect of rice husk and polypropylene on compressive *
*and split tensile strength of M20 concrete. Rice husk ash and *
*polypropylene have been mixed with concrete in combination *
*in different proportions. Rice husk has been used in 2.5%, 5% *
*&10% by weight of cement. Polypropylene fiber content varies *
*from 0%, 0.25%, 0.5% &0.75% by weight of concrete. We can *
*see the maximum strength value by plotting the test result of *
*cube for compressive strength test and cylinder for split tensile *
*strength test for 7days and 28 days. At 10% rice husk and *
*0.5% polypropylene 7 days peak compressive strength has *
*been achieved which is 22.6% higher than controlled concrete. *
*At 5% rice husk and 0.5% polypropylene fiber 7 days peak split *
*tensile strength has been achieved which is 53.57% higher *
*than controlled concrete. At 10% rice husk ash and 0.5% *
*polypropylene fiber 28 days peak compressive strength has *
*been achieved which is 54.61% higher than controlled *
*concrete. At 5% rice husk and 0.5% polypropylene fiber 28 *
*days peak split tensile strength has been achieved which is *
*31.34% higher than controlled concrete. *

**Key Words****:** Rice Husk Ash, Polypropylene Fiber,
Compressive Strength, Split Tensile Strength, ordinary
Portland cement (OPC).

**1. INTRODUCTION **

In India, rice milling produces a by product which is also known as husk. Rice husk is a waste material, and has been disposed of by dumping or burning. By using rice husk ash in concrete, we can improve the properties of concrete up to some extent. RHA is found to be good material which fulfils the physical characteristics and chemical composition of mineral admixtures. A small amount of addition of RHA (less than 10 % by weight of cement), is sufficient to improve the durability as well as the strength of concrete. RHA contain high silica content that reduces shrinkage and leads to increases in the strength of concrete

Polypropylene fiber are synthetic fiber obtain as a by product from textile industry. Polypropylene fiber is characterized by low specific gravity and low cost. The use of

polypropylene fiber has increased tremendously in construction because it behaves like reinforcement. Addition of polypropylene fiber in concrete improves the compressive and tensile strength of concrete. The addition of polypropylene fibers in the concrete significantly affects the compressive strength and split tensile strength of concrete. Addition of polypropylene fiber in concrete increases the compressive strength by 20% to 55% and splitting tensile strength by 30% to 50% respectively. In this study the influence of different amount of rice husk ash and polypropylene fibers content on concrete properties were investigated by measuring compressive strength and splitting tensile strength.

**1.1** **Objectives **

The main purpose of this project is to investigate mechanical properties of rice husk ash cement concrete with the addition of polypropylene fiber. Mainly following objectives are considered-

1. To study the properties of fresh and hardened concrete.

2. To study the physical and chemical properties of raw material.

3. To investigate how much percentage of rice husk ash and polypropylene fiber improve mechanical properties of concrete.

4. To study the improvement of split tensile strength of concrete by using rice husk ash and polypropylene fiber.

5. To study the improvement of compressive strength of concrete by using rice husk ash and polypropylene fiber.

6. To study the cost analysis by using RHA and polypropylene fiber.

**1.2** **Planning For Experiment **

**2. MIX DESIGN **

The M20 grade concrete generally used for general purpose, For concrete mix design raw material are collected from resources with specified specifications and quality. All the materials are tested as per IS code. In previous time concrete mixed design conforms to IS 456-2000 but in present time with latest provisions concrete mix design calculation has been done as per as per IS 10262-2009.

**Step1.** Data required for mix proportioning –

**S.No. ** **Characteristic properties ** **Values **

1 Grade of concrete M -20

2 Maximum nominal size of

aggregates 20mm

3 Grade of cement OPC 53

grade 4 Specific gravity of fine

aggregate 2.65

5 Maximum water-cement

ratio 0.5

6 Workability (for slump test) 100 mm 7 Grading Zone of fine

aggregate Zone-II

8 Specific gravity of cement 3.15 9 Specific gravity of coarse

aggregate 2.68

10 Aggregate shape Angular

11 Entrapped air 2.00%

12 Admixture used Nil

13 Maximum temperature of concrete at the time of

pouring

27 ± 2°C

14 Minimum cement content 450 kg/m³ 15 Minimum cement content 300 kg/m³ 16 Surface moisture – fine

aggregates & coarse aggregates

Nil

17 Method of transporting &

placing Manual

18 Exposure conditions

IS-456:2009 Table no 4 Mild

**Step2**. Calculation of target mean strength = 26.6 N/mm²

**Step3**. Calculation or selection of water cement ratio = 0.48
**Step4**. Calculation of water content = 197.16 litre/m3

**Step5**. Calculation of cement content = 411kg/m3
**Step6**. Calculation of mix proportion

Mass of coarse aggregate = 1134 kg/m³ Mass of fine aggregate = 670 kg/m³

**Step7**. Final Mix proportion by weight for trial mix:

**Water ** **Cement Fine aggregate ** **Coarse aggregate **

197 411 kg 670 kg 1134 kg

0.48 1 1.63 2.75

**3. TEST ON CONCRETE **

** 3.1 Compressive Strength Test **

The compressive strength test for concrete specimens has been performed in Compression Testing Machine (CTM) having maximum loading capacity of 2000KN. 30 concrete specimens were tested for 7 days compressive strength and 30 concrete specimens were tested for 28 days compressive strength.

Fig. 3.1: Compression testing Machine

**3.2 Split Tensile Strength Test **

The split tensile strength test for concrete specimens has been performed in Split Tensile Testing Machine. 30 concrete specimens were tested for 7 days split tensile strength and 30 concrete specimens were tested for 28 days split tensile strength.

Fig. 3.2: Universal testing Machine

**S.N. ** **BATCHES ** **DISCRIPTION **

**(CEMENT+RICE RICE HUSK ASH + **
**POLYPROPYLENE FIBER) **

01. M-1 100+0+0

O2. M-2 97.5+2.5+0.25

03. M-3 97.5+2.5+0.50

04. M-4 97.5+2.5+0.75

05. M-5 95+5+0.25

06. M-6 95+5+0.50

07. M-7 95+5+0.75

08. M-8 90+10+0.25

09. M-9 90+10+0.50

**4. CALCULATION OF NUMBER OF CUBE AND CYLINDER **
**SPECIMEN REQUIRED: **

**5. RESULT AND DISSCUSION **
**5.1 Compressive Strength **
**7 Days Compressive Strength **

0 5 10 15 20 25

Controlled 2.5% Rice
Husk
5% Rice
Husk
10% Rice
Husk
A
ve
ra
ge
Co
mpr
es
si
ve
S
tr
ength
(N
/mm2
**)**

Percentage of Rice Husk And Polypropylene 0.25% Polypropyl ene 0.5% Polypropyl ene 0.75% Polypropyl ene

Fig 5.1.1: 7 Days compressive strength

For 7 days compressive strength, the peak strength was
obtained as 21.37N/mm**2**_{ from concrete containing 10% rice }
husk ash + 0.5% Polypropylene fiber which was 22.6%
higher than compressive strength of controlled concrete
(17.43N/mm**2**_{). It is also observed that for concrete }
containing 0.25% Propylene fiber + 2.5% rice husk ash,
compressive strength was little higher than controlled
concrete. But further increase in rice husk ash percentage
compressive strength decreased. For 0.5% Polypropylene
fiber + 2.5% rice husk ash compressive strength was little
higher than controlled concrete. But with increase in rice
husk ash, compressive strength also increased. For 0.75%
polypropylene fiber + 2.5% rice husk ash compressive
strength was lesser than controlled concrete. But with
increase in rice husk ash compressive strength also increased

but could reach equal to compressive strength of controlled concrete.

**28 days Compressive strength **

0
5
10
15
20
25
30
35
40
45
A
ve
ra
ge
C
om
pr
es
si
ve
S
tr
en
gt
h
(N
/m
m
2
**)**

Percentage of Rice Husk And Polypropylene 0.25% Polypropy lene 0.5% Polypropy lene

Fig 5.1.2: 28 Days compressive strength

For 28 days compressive strength the peak strength was
obtained as 42.055N/mm**2**_{ from concrete containing 10% }
rice husk ash + 0.5% Polypropylene fiber which was 54.6%
higher than compressive strength of controlled concrete
(27.2N/mm**2**_{). It is also observed that for 0.25% }
polypropylene fiber + 2.5% rice husk ash compressive
strength was significantly higher than controlled concrete.
But further increase in rice husk ash percentage compressive
strength decreased, but always higher than compressive
strength of controlled concrete. For 0.5% polypropylene fiber
+ 2.5% rice husk ash compressive strength was significantly
higher than controlled concrete. But with increase in rice
husk ash compressive strength also increased. For 0.75%
polypropylene fiber + 2.5% rice husk ash compressive
strength was little higher than controlled concrete. But with
increase in rice husk ash compressive strength also
increased.

**5.2 Split tensile strength **
**7 days Split tensile strength **

0 0.5 1 1.5 2 2.5 3

Controlled 2.5% Rice

Husk 5% RiceHusk 10% RiceHusk

A
ve
ra
ge
C
om
pr
es
si
ve
S
tr
en
gt
h
(N
/m
m
2
**)**

Percentage of Rice Husk And Polypropylene 0.25% Polypropy lene 0.5% Polypropy lene 0.75% Polypropy lene

Fig 5.2.1: 7 Days split tensile strength Sample

No % of rice husk ash % of polyp ropyl ene

No of cube No of cylinder 7 days test 28 days test 7 days test 28 days test

1. 0 0 3 3 3 3

2. 2.5 0.25 3 3 3 3

3. 2.5 0.5 3 3 3 3

4. 2.5 0.75 3 3 3 3

5. 5 0.25 3 3 3 3

6. 5 0.5 3 3 3 3

7. 5 0.75 3 3 3 3

8. 10 0.25 3 3 3 3

9. 10 0.5 3 3 3 3

10. 10 0.75 3 3 3 3

Sub Total 30 30 30 30

For 7 days split tensile strength the peak strength was
obtained as 2.58N/mm**2 **_{from concrete containing 5% rice }
husk ash + 0.5% Polypropylene fiber which was 53.57%
higher than compressive strength of controlled concrete
(1.68N/mm**2**_{). It is also observed that for 2.5% rice husk ash }
split tensile strength was lesser than split tensile strength of
controlled concrete for every percentage of Polypropylene
fiber. For 5% rice husk ash split tensile strength was
significantly higher than split tensile strength of controlled
concrete for every percentage of Polypropylene fiber. For
10% rice husk ash split tensile strength was lesser than split
tensile strength of controlled concrete for all proportions of
Polypropylene fiber

**28 Days Split tensile strength **

For 28 days split tensile strength the peak strength was
obtained as 3.31N/mm**2 **_{from concrete contained 5% rice }
husk ash + 0.5% Polypropylene fiber which was 31.3%
higher than compressive strength of controlled concrete
(2.52N/mm**2**_{). It is also observed that for 2.5% rice husk ash }
split tensile strength was lesser than split tensile strength of
controlled concrete for every percentage of Polypropylene
fiber. For 5% rice husk ash split tensile strength was higher
than split tensile strength of controlled concrete for every
percentage of Polypropylene fiber. For 10% rice husk ash
split tensile strength was significantly lesser than split
tensile strength of controlled concrete for every percentage
of Polypropylene fiber.

0 0.5 1 1.5 2 2.5 3 3.5

Controlled 2.5% Rice

Husk 5% Rice Husk 10% Rice Husk

Ave

rag

e

Co

mpr

essiv

e

St

reng

th

(

N/

mm

2

**)**

Percentage of Rice Husk And Polypropylene

0.25% Polypropyl ene 0.5% Polypropyl ene 0.75% Polypropyl ene

Fig 5.2.2: 28 Days split tensile strength

**6. CONCLUSIONS **

From all the result and discussions following conclusions can be made:-

i) Addition of rice husk and Polypropylene in concrete improves characteristic compressive and split tensile strength.

ii) Optimum dosage of rice husk can be taken from 5% by weight of cement.

iii) Optimum dosage of Polypropylene fiber can be taken from 0.5% by weight of concrete.

iv) Maximum increase in compressive strength for 7 and 28 days is 22.6% and 54.61% respectively as compare to control concrete.

v) Maximum increase in split tensile strength for 7 and 28 days is 53.57% and 31.34% respectively as compare to control concrete.

vi) For 7 days compressive strength test the concrete containing 0.5% PPF gives greater strength as compare to control concrete for every percentage of RHA. vii) For 28 days compressive strength test the concrete

containing 0.25%, 0.5% and 0.75% PPF gives greater strength as compare to control concrete for every percentage of RHA.

viii) Cost of per cubic meter concrete containing 5% rice husk + 0.5% polypropylene is Rs2778.44 which is Rs19.1 lesser than cost of per cubic meter controlled concrete.

From above points it is clear that concrete containing 5% rice husk and 0.5% Polypropylene achieves significantly higher characteristic compressive and split tensile strength as compare to controlled concrete with economy. So according to this experimental study the recommended dosage of rice husk and Polypropylene fiber is 5% and 0.5% respectively.

**REFERENCES **

1. Alsadey Salahaldein (2016) “Effect of Polypropylene Fiber Reinforced on Properties of Concrete” Journal of Advance Research in Civil and Mechanical Engineering. 2. Arivalagan S,(2014) “Earthquake-Resistant Performance of Polypropylene Fiber Reinforced Concrete beams ”, Journal of Engineering and Technology, Vol. 2 (01),pp. 63-67

3. Aly T Sanjayan G and Collins F,( 2014) “ Effect of
Polypropylene Fiber on shrinkage and cracking of
concretes”,Journal of materials and structure, Vol. 2
(01)** , **pp1471-1753** **

4. Cengiz, O and Turanil, L (2004). “Comparative evaluation of steel mesh, steel fiber and High performance polypropylene fiber reinforced shotcrete in panel tests”, Cement and Research. Vol.34, Jan .pp 1357-1364.

5. Dave U. V. and Desai Y. M (2007) “ Effect of Polypropylene, Polyester and Glass Fiber on various strength of ordinary and standard concrete”, The First International Conference On Recent Advance in Concrete Technology, Washington D.C.U.S.A.

6. IS: 456-2000, Indian standard, “PLAIN AND REINFORCED CONCRETE CODE OF PRACTICE”, (Fourth Revision).

8. IS: 12269-2013, Indian standard, “ORDINARY PORTLAND CEMENT, 53 GRADE-SPECIFICATION” (First Revision).

9. IS: 516-1959, Indian standard, “MEHTOD OF TEST FOR STRENGTH OF CONCRETE”

10. IS: 383-1970, Indian standard, “SPECIFICATION FOR COARSE AND FINE AGGREGATE FROM NATURAL SOURCES FOR CONCRETE”

11. Kishore, R., Bhikshma, V. and Prakash, P.J. (2011) “Study on Strength Characteristics of High Strength Rice Husk Ash Concrete”, Procedia Engineering 14, pp. 266-26

12. Market study of Polypropylene (3rd_{ edition) Ceresana. }
13. Nagrale, S.D., Hazare, H. and Modak, P.R. (2012)

“Utilization of Rice Husk Ash”, International Journal of Engineering Research and

Applications (IJERA). Vol. 2, Issue 4, pp. 001-005 14. Shetty, M.S. (2012) Concrete.S. Technology. S. Chand

Publication New Delhi.

15. Zhang, M.H., Lastra, R. and Malhotra, V.M. (1996) “Rice Husk Ash Paste and Concrete: Some Aspects of Hydration and the microstructure of the Interfacial Zone between the Aggregate and Paste”, Cement and concrete Research, Vol. 26, No. 6, pp. 963-977. 16. Zhang, M.H., & Malhotra, V. M. (1996) “High-